Cu~12~Sb~4~S~13~: A Temperature-Dependent Structure Investigation
Pfitzner, A.; Evain, M.; Petricek, V.; Acta Crystallographica Section B 53 (1997) 337–345; doi:10.1107/S0108768196014024

data_2101864
_publ_section_title
;
 Cu~12~Sb~4~S~13~: A Temperature-Dependent Structure Investigation
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              337
_journal_page_last               345
_journal_paper_doi               10.1107/S0108768196014024
_journal_volume                  53
_journal_year                    1997
_chemical_formula_sum            'Cu12 S13 Sb4'
_chemical_formula_weight         1666.33
_space_group_IT_number           217
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_atom_type_scat_source           IntTabIV
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   10.3293(6)
_cell_length_b                   10.3293(6)
_cell_length_c                   10.3293(6)
_cell_measurement_reflns_used    26
_cell_measurement_temperature    295
_cell_measurement_theta_max      15.4
_cell_measurement_theta_min      5.4
_cell_volume                     1102.08(11)
_diffrn_measurement_device       'Siemens P4'
_diffrn_measurement_method       'Profile-fitted \w'
_diffrn_radiation_type           AgK-L~2,3~
_diffrn_radiation_wavelength     0.56087
_diffrn_reflns_av_R_equivalents  0.041
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            3000
_diffrn_reflns_theta_max         27.96
_diffrn_standards_decay_%        <1
_diffrn_standards_interval_count 100
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    8.973
_exptl_absorpt_correction_T_max  0.82
_exptl_absorpt_correction_T_min  0.61
_exptl_absorpt_correction_type   '\y-scan (Sheldrick, 1996)'
_exptl_crystal_colour            'metallic black'
_exptl_crystal_density_diffrn    5.020
_exptl_crystal_description       irregular
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.72
_refine_diff_density_min         -0.85
_refine_ls_extinction_coef       0.270(10)
_refine_ls_extinction_method     'Secondary isotropic'
_refine_ls_goodness_of_fit_obs   1.11
_refine_ls_number_parameters     34
_refine_ls_number_reflns         389
_refine_ls_R_factor_obs          0.0165
_refine_ls_shift/esd_max         <0.0001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     'w = 1/[\s^2^(|F~o~|) + (0.01|F~o~|)^2^]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_obs         0.0200
_reflns_number_observed          389
_reflns_number_total             538
_reflns_observed_criterion       I>1\s(I)
_cod_data_source_file            se0205.cif
_cod_data_source_block           se0205a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'w = 1/[\s^2^(|F~o~|) +
(0.01|F~o~|)^2^]' was changed to 'calc'. New tag
'_refine_ls_weighting_details' was created. The value of the new tag
was set to 'w = 1/[\s^2^(|F~o~|) + (0.01|F~o~|)^2^]'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        1102.1(2)
_cod_database_code               2101864